Cell-adhesive RGD peptide-displaying M13 bacteriophage/PLGA nanofiber matrices for growth of fibroblasts
- Yong Cheol Shin†1,
- Jong Ho Lee†1,
- Linhua Jin1,
- Min Jeong Kim1,
- Jin-Woo Oh2,
- Tai Wan Kim3 and
- Dong-Wook Han1Email author
© Shin et al.; licensee BioMed Central Ltd. 2014
Received: 3 July 2014
Accepted: 29 August 2014
Published: 3 October 2014
M13 bacteriophages can be readily fabricated as nanofibers due to non-toxic bacterial virus with a nanofiber-like shape. In the present study, we prepared hybrid nanofiber matrices composed of poly(lactic-co-glycolic acid, PLGA) and M13 bacteriophages which were genetically modified to display the RGD peptide on their surface (RGD-M13 phage).
The surface morphology and chemical composition of hybrid nanofiber matrices were characterized by scanning electron microscopy (SEM) and Raman spectroscopy, respectively. Immunofluorescence staining was conducted to investigate the existence of M13 bacteriophages in RGD-M13 phage/PLGA hybrid nanofibers. In addition, the attachment and proliferation of three different types of fibroblasts on RGD-M13 phage/PLGA nanofiber matrices were evaluated to explore how fibroblasts interact with these matrices. SEM images showed that RGD-M13 phage/PLGA hybrid matrices had the non-woven porous structure, quite similar to that of natural extracellular matrices, having an average fiber diameter of about 190 nm. Immunofluorescence images and Raman spectra revealed that RGD-M13 phages were homogeneously distributed in entire matrices. Moreover, the attachment and proliferation of fibroblasts cultured on RGD-M13 phage/PLGA matrices were significantly enhanced due to enriched RGD moieties on hybrid matrices.
These results suggest that RGD-M13 phage/PLGA matrices can be efficiently used as biomimetic scaffolds for tissue engineering applications.
KeywordsM13 bacteriophages RGD peptide PLGA nanofibers Extracellular matrices Fibroblasts
In the body, most cells grow on the extracellular matrix (ECM) which is porous structure consisting of fibrous proteins and glycosaminoglycans. The ECM is the outer parts of cells in tissues and provides an essential environment for cells to survive. The ECM is very important because it affects cellular behaviors such as cell adhesion, proliferation and differentiation through biochemical or physical signal as well as provides a 3D microenvironment conductive to cellular growth [1–4]. Recently, many efforts are under way to develop a biomimetic artificial ECM for tissue engineering applications by using various biodegradable polymers [5–7]. Poly(lactic-co-glycolic acid, PLGA), as one of synthetic biodegradable polymers, has been most extensively used in drug delivery and scaffold applications due to its excellent biocompatibility and suitable physicochemical properties [8–11]. Among many biomolecules within the ECM, adhesive proteins such as fibronectin and laminin play an important role in cellular attachment and proliferation. Generally, most of animal cells attach to the ECM through direct interaction between transmembrane integrin receptor and adhesive proteins. The primary sequence motif of fibronectin for integrin binding is a tripeptide, Arg-Gly-Asp (RGD [12–14]. Therefore, matrices which are enriched with RGD peptides promote not only cellular attachment but also cellular behaviors [15, 16].
An electrospinning technique has been widely used to fabricate nanofibrous matrices which were structurally similar to the natural ECM. A previous study has already shown that nanofibrous matrices fabricated by an electrospinning process were suitable for tissue engineering scaffolds . The advantage of this technique is that non-woven porous matrices can be easily produced as well as incorporated with bioactive agents including growth factors, peptides and drugs .
M13 bacteriophage is bacterial virus with nanofiber-like shaped [18, 19]. Moreover, M13 bacteriophages do not have any detrimental effect on mammalian cells [20–22]. Some previous studies showed that M13 bacteriophage could express many desired proteins on their surface [23–25]. In addition, M13 bacteriophages can be readily fabricated as nanofibers via an electrospinning process due to their structural property .
The aim of the present study was to fabricate RGD peptide-displaying M13 bacteriophages (RGD-M13 phages)/PLGA hybrid nanofiber matrices to mimic the natural ECM by electrospinning. We showed that RGD-M13 phage/PLGA hybrid matrices were successfully fabricated and RGD-M13 phages were uniformly distributed over the matrices. Furthermore, we examined cellular behaviors of fibroblasts on RGD-M13 phage/PLGA nanofiber matrices to explore how the cells interact with these matrices. As a result, we demonstrated that these matrices improved cellular behaviors by synergistic effects, resulting from the excellent biocompatibility of PLGA and the ability to enhance the cell attachment of RGD sequences displayed on the surface of M13 bacteriophages. Therefore, this result implies that RGD-M13 phage/PLGA hybrid matrices can be one of the best potential candidates for biomimetic tissue engineering scaffolds.
Fabrication of RGD-M13 phage/PLGA nanofibers by electrospinning
Characterizations of RGD-M13 phage/PLGA hybrid nanofibers
The surface morphology of RGD-M13 phage/PLGA matrices was observed under a scanning electron microscope (SEM). The matrices were coated with an ultrathin layer of gold/platinum by an ion sputter (E1010, Hitach, Tokyo, Japan) prior to analysis. The RGD-M13 phages and nanofibers were characterized by using Raman spectroscopy. For immunofluorescence staining to examine whether M13 bacteriophages exist in RGD-M13 phage/PLGA matrices or not, the matrices were incubated with primary anti-M13 bacteriophage antibody [at 1:250 in 2% bovine serum albumin (BSA) solution in phosphate-buffered saline (PBS, pH 7.4); Sigma-Aldrich] for 2 h at room temperature and then incubated with secondary FITC-conjugated goat anti-rabbit IgG (at 1:500 in 2% BSA solution in PBS; Abcam Inc., Cambridge, MA) for 1 h at room temperature. Immunostained matrices were imaged with an Olympus IX81 inverted fluorescence microscope (Olympus Optical Co., Osaka, Japan).
Cells and culture conditions
In the present study, three different types of fibroblasts were employed – two types were immortalized and cancerous cell lines and one was a primary cell. Murine fibroblasts (L-929 cells) and human fibrosarcoma cells (HT-1080 cells) were purchased from American Type Culture Collection (ATCC, Rockville, MD) and routinely maintained in Dulbecco’s modified Eagle’s Medium (DMEM, Welgene, Daegu, Korea). Human dermal fibroblasts (HDFs) from neonatal dermis were kindly provided by Dr. Dong Kyun Rah (Department of Plastic and Reconstructive Surgery, Yonsei University College of Medicine, Seoul, Korea) and cultured in fibroblast basal medium (FBM, Lonza, Basel, Switzerland). All cells were cultured in complete media supplemented with 10% fetal bovine serum (FBS, Welgene) and 1% antibiotic-antimycotic solution (including 10,000 units penicillin, 10 mg streptomycin and 25 μg amphotericin B per ml, Sigma-Aldrich, St. Louis, MO) at 37°C in a humidified atmosphere containing 5% CO2.
In vitroassays for fibroblast behaviors on RGD-M13 phage/PLGA nanofibers
Cell attachment and proliferation were measured by using a cell counting kit-8 (CCK-8, Dojindo, Kumamoto, Japan), which contains highly water-soluble tetrazolium salt [WST-8, 2-(2-methoxy-4-nitrophenyl)-3-(4-nitrophenyl)-5-(2,4-disulfophenyl)-2H-tetrazolium, monosodium salt], reduced to a water-soluble formazan dye by dehydrogenases in cells. The number of viable cells was found to be directly proportional to the metabolic reaction products obtained in the CCK-8 assay . Typically, three types of fibroblasts were seeded at a density of 1 × 104 cells/mL on PLGA or RGD-M13 phage/PLGA matrices. According to the manufacturer’s instruction, each cell culture was incubated with a WST-8 solution in the last 4 hours of culture periods for cell attachment (6 hours) or proliferation (1, 3, 5 and 7 days) at 37°C in the dark. Parallel sets of cells cultured on tissue culture plastics (TCP) were regarded as controls. The absorbance was determined at 450 nm by an ELISA reader (SpectraMax 340, Molecular Device Co., Sunnyvale, CA). For morphological observations, HDFs cultured on matrices for 3 days were fixed with 3.7% formaldehyde solution (Sigma-Aldrich) for 10 minutes. After fixation, HDF-cultured matrices were dehydrated in a graded series of ethanol, followed by air-drying overnight. The matrices were sputter-coated with gold/platinum and then observed under a scanning electron microscope (SEM, Hitachi S-800, Tokyo, Japan) at an accelerating voltage of 5 kV.
All variables were tested in three independent cultures for each experiment, which was repeated twice (n = 6). Quantitative data are expressed as the mean ± standard deviation (SD). Data were tested for homogeneity of variances using the test of Levene, prior to statistical analysis. Multiple comparisons to detect the cellular behaviors on RGD-M13 phage/PLGA nanofiber matrices were carried out using one-way analysis of variance (ANOVA, SAS Institute, Cary, NC), which was followed by the Bonferroni test when variances were homogeneous and the Tamhane test when variances were not. A value of p < 0.05 was considered statistically significant.
Results and discussion
Physicochemical characteristics of RGD-M13 phage/PLGA hybrid nanofibers
Fibroblast behaviors on RGD-M13 phage/PLGA nanofiber matrices
This study was designed to fabricate RGD-M13 phage/PLGA hybrid matrices that could applied for tissue engineering scaffolds. The suitable scaffold should be biocompatible and biodegradable. In addition, its structure should have a porous structure which is analogous to the natural ECM in order to support the growth of cells. We successfully fabricated the RGD-M13 phage/PLGA matrices by using electrospinning and analyzed various properties of them. Results showed that the hybrid matrices had outstanding biocompatibility and suitable physicochemical properties as well as structurally comparable to the natural ECM. Moreover, they were biofunctional scaffolds which could effectively improve cellular attachment and proliferation through RGD peptides existed along the nanofibers. Based on these results, RGD-M13 phage/PLGA hybrid matrices had a high probability to use for biodegradable scaffolds. In summary, it is suggested that the RGD-M13 phage/PLGA hybrid matrices can be employed to bioactive scaffolds for tissue engineering application.
Availability of supporting data
There was no available supporting data.
This study was supported by Basic Science Research Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education, Science and Technology (2012R1A2A2A02010181).
- Ingber DE, Folkman J: Mechanochemical switching between growth and differentiation during fibroblast growth factor-stimulated angiogenesis in vitro: role of extracellular matrix. J Cell Biol. 1989, 109: 317-330. 10.1083/jcb.109.1.317.View ArticleGoogle Scholar
- Juliano RL, Haskill S: Signal transduction from the extracellular matrix. J Cell Biol. 1993, 120: 577-585. 10.1083/jcb.120.3.577.View ArticleGoogle Scholar
- Meredith JE, Fazeli B, Schwartz MA: The extracellular matrix as a cell survival factor. Mol Biol Cell. 1993, 4: 953-961. 10.1091/mbc.4.9.953.View ArticleGoogle Scholar
- Thery M, Racine V, Pepin A, Piel M, Chen Y, Sibarita JB, Bornens M: The extracellular matrix guides the orientation of the cell division axis. Nat Cell Biol. 2005, 7: 947-953. 10.1038/ncb1307.View ArticleGoogle Scholar
- Mo XM, Xu CY, Kotaki M, Ramakrishna S: Electrospun P(LLA-CL) nanofiber: a biomimetic extracellular matrix for smooth muscle cell and endothelial cell proliferation. Biomaterials. 2004, 25: 1883-1890. 10.1016/j.biomaterials.2003.08.042.View ArticleGoogle Scholar
- Fujihara K, Kotaki M, Ramakrishna S: Guided bone regeneration membrane made of polycaprolactone/calcium carbonate composite nano-fibers. Biomaterials. 2005, 26: 4139-4147. 10.1016/j.biomaterials.2004.09.014.View ArticleGoogle Scholar
- Zhang YZ, Su B, Venugopal J, Ramakrishna S, Lim CT: Biomimetic and bioactive nanofi brous scaffolds from electrospun composite nanofibers. Int J Nanomed. 2007, 2: 623-638.Google Scholar
- Beletsi A, Leontiadis L, Klepetsanis P, Ithakissios DS, Avgoustakis K: Effect of preparative variables on the properties of poly(dl-lactide-co-glycolide)–methoxypoly(ethyleneglycol) copolymers related to their application in controlled drug delivery. Int J Pharm. 1999, 182: 187-197. 10.1016/S0378-5173(99)00058-7.View ArticleGoogle Scholar
- Ravichandran R, Ng CC, Liao S, Pliszka D, Raghunath M, Ramakrishna S, Chan CK: Biomimetic surface modification of titanium surfaces for early cell capture by advanced electrospinning. Biomed Mater. 2012, 7: 015001-10.1088/1748-6041/7/1/015001.View ArticleGoogle Scholar
- Wei K, Li Y, Lei X, Yang H, Teramoto A, Yao J, Abe K, Ko FK: Emulsion electrospinning of a collagen-like protein/PLGA fibrous scaffold: Empirical modeling and preliminary release assessment of encapsulated protein. Macromol Biosci. 2011, 11: 1526-1536.Google Scholar
- Chen DW, Hsu YH, Liao JY, Liu SJ, Chen JK, Ueng SW: Sustainable release of vancomycin, gentamicin and lidocaine from novel electrospun sandwich-structured PLGA/collagen nanofibrous membranes. Int J Pharm. 2012, 430: 335-341. 10.1016/j.ijpharm.2012.04.010.View ArticleGoogle Scholar
- Pytela R, Pierschbacher MD, Ginsberg MH, Plow EF, Ruoslahti E: Platelet membrane glycoprotein IIb/IIIa: member of a family of Arg-Gly-Asp-specific adhesion receptors. Science. 1986, 231: 1559-1562. 10.1126/science.2420006.View ArticleGoogle Scholar
- Ruoslahti E, Pierschbacher MD: New perspectives in cell adhesion: RGD and integrins. Science. 1987, 238: 491-497. 10.1126/science.2821619.View ArticleGoogle Scholar
- Staatz WD, Fok KF, Zutter MM, Adams SP, Rodriguez BA, Santoro SA: Identification of a tetrapeptide recognition sequence for the α2β1 integrin in collagen. J Biol Chem. 1991, 266: 7363-7367.Google Scholar
- Ho MH, Wang DM, Hsieh HJ, Liu HC, Hsien TY, Lai JY, Ho LT: Preparation and characterization of RGD-immobilized chitosan scaffolds. Biomaterials. 2005, 26: 3197-3206. 10.1016/j.biomaterials.2004.08.032.View ArticleGoogle Scholar
- Zhang L, Hum M, Wang M, Li Y, Chen H, Chu C, Jiang H: Evaluation of modifying collagen matrix with RGD peptide through periodate oxidation. J Biomed Mater Res A. 2005, 73A: 468-475. 10.1002/jbm.a.30363.View ArticleGoogle Scholar
- Lee J, Cuddihy MJ, Kotov NA: Three-dimensional cell culture matrices: state of the art. Tissue Eng Part B. 2008, 14: 61-86. 10.1089/teb.2007.0150.View ArticleGoogle Scholar
- Smith GP, Petrenko VA: Phage display. Chem Rev. 1997, 97: 391-410. 10.1021/cr960065d.View ArticleGoogle Scholar
- Dogic Z, Fraden S: Smectic phase in a colloidal suspension of semiflexible virus particles. Phys Rev Lett. 1997, 78: 2417-2420. 10.1103/PhysRevLett.78.2417.View ArticleGoogle Scholar
- Frenkel D, Solomon B: Filamentous phage as vector-mediated antibody delivery to the brain. Proc Natl Acad Sci U S A. 2002, 99: 5675-5679. 10.1073/pnas.072027199.View ArticleGoogle Scholar
- Yoo SY, Kobayashi M, Lee PP, Lee SW: Early osteogenic differentiation of mouse preosteoblasts induced by collagen-derived DGEA-peptide on nanofibrous phage tissue matrices. Biomacromolecules. 2011, 12: 987-996. 10.1021/bm1013475.View ArticleGoogle Scholar
- Zhu H, Cao B, Zhen Z, Laxmi AA, Li D, Liu S, Mao C: Controlled growth and differentiation of MSCs on grooved films assembled from monodisperse biological nanofibers with genetically tunable surface chemistries. Biomaterials. 2011, 32: 4744-4752. 10.1016/j.biomaterials.2011.03.030.View ArticleGoogle Scholar
- Chung WJ, Oh JW, Kwak K, Lee BY, Meyer J, Wang E, Hexemer A, Lee SW: Biomimetic self-templating supramolecular structures. Nature. 2011, 478: 364-368. 10.1038/nature10513.View ArticleGoogle Scholar
- Wang J, Wang L, Li X, Mao C: Virus activated artificial ECM induces the osteoblastic differentiation of mesenchymal stem cells without osteogenic supplements. Sci Rep. 2013, 3: 1242-Google Scholar
- Merzlyak A, Indrakanti S, Lee SW: Genetically engineered nanofiber-like viruses for tissue regenerating materials. Nano Lett. 2009, 9: 846-852. 10.1021/nl8036728.View ArticleGoogle Scholar
- Lee SW, Belcher AM: Virus-based fabrication of micro- and nanofibers using electrospinning. Nano Lett. 2004, 4: 387-390. 10.1021/nl034911t.View ArticleGoogle Scholar
- Chen G, Courey AJ: Generation of epitope-tagged proteins by inverse PCR mutagenesis. Biotechniques. 1999, 26: 814-816.Google Scholar
- Qi D, Scholthof KB: A one-step PCR-based method for rapid and efficient site-directed fragment deletion, insertion, and substitution mutagenesis. J Virol Methods. 2008, 149: 85-90. 10.1016/j.jviromet.2008.01.002.View ArticleGoogle Scholar
- Lee EJ, Lee JH, Shin YC, Hwang DG, Kim JS, Jin OS, Jin L, Hong SW, Han DW: Graphene oxide-decorated PLGA/collagen hybrid fiber sheets for application to tissue engineering scaffolds. Biomater Res. 2014, 18: 18-24.View ArticleGoogle Scholar
- Atabaev TS, Jin OS, Lee JH, Han DW, Vu HHT, Hwang YH, Kim HK: Facile synthesis of bifunctional silica-coated core–shell Y2O3:Eu3+, Co2+ composite particles for biomedical applications. RSC Adv. 2012, 2: 9495-9501. 10.1039/c2ra21332j.View ArticleGoogle Scholar
- Stewart S, Fredericks PM: Surface-enhanced Raman spectroscopy of amino acids adsorbed on an electrochemically prepared silver surface. Spectrochim Acta A. 1999, 55: 1641-1660. 10.1016/S1386-1425(98)00294-7.View ArticleGoogle Scholar
- Apeldoorn AA, Manen HJ, Bezemer JM, Bruijn JD, Blitterswijk CA, Otto C: Raman imaging of PLGA microsphere degradation inside macrophages. J Am Chem Soc. 2004, 126: 13226-13227. 10.1021/ja0459936.View ArticleGoogle Scholar
- Filho PF, Freire PTC, Lima KCV, Filho JM, Melo FEA, Pizani PS: High temperature raman spectra of L-leucine crystals. Braz J Phys. 2008, 38: 131-137. 10.1590/S0103-97332008000100024.View ArticleGoogle Scholar
- Hersel U, Dahmen C, Kessler H: RGD modified polymers: biomaterials for stimulated cell adhesion and beyond. Biomaterials. 2003, 24: 4385-4415. 10.1016/S0142-9612(03)00343-0.View ArticleGoogle Scholar
- Bellis SL: Advantages of RGD peptides for directing cell association with biomaterials. Biomaterials. 2011, 32: 4205-4210. 10.1016/j.biomaterials.2011.02.029.View ArticleGoogle Scholar
- Tsai WB, Chen YR, Liu HL: RGD-conjugated crosslinked chitosan scaffolds for culture and osteogenic differentiation of mesenchymal stem cells. J Taiwan Inst Chem E. 2013, 44: 17-Google Scholar
- Shin YM, Jo SY, Park JS, Gwon HJ, Jeong SI, Lim YM: Synergistic effect of dual-functionalized fibrous scaffold with BCP and RGD containing peptide for improved osteogenic differentiation. Macromol Biosci. 2014, doi:10.1002/mabi.201400023Google Scholar
- Masaeli E, Wieringa PA, Morshed M, Nasr-Esfahani MH, Sadri S, Blitterswijk CA, Moroni L: Peptide functionalized polyhydroxyalkanoate nanofibrous scaffolds enhance Schwann cells activity. Nanomedicine. 2014, doi:10.1016/j.nano.2014.04.008Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.